# drag reduction behavior of hydrolyzed polyacrylamide

Embed Size (px)

TRANSCRIPT

Drag reduction behavior of hydrolyzed polyacrylamide/xanthan gum
mixed polymer solutionsMehdi Habibpour1 • Peter E. Clark1

Received: 6 October 2016 / Published online: 28 March 2017

The Author(s) 2017. This article is an open access publication

Abstract Partially hydrolyzed polyacrylamide (HPAM) as

the main component of slickwater fracturing fluid is a

shear-sensitive polymer, which suffers from mechanical

degradation at turbulent flow rates. Five different concen-

trations of HPAM as well as mixtures of polyacrylamide/

xanthan gum were prepared to investigate the possibility of

improving shear stability of HPAM. Drag reduction (DR)

measurements were performed in a closed flow loop. For

HPAM solutions, the extent of DR increased from 30% to

67% with increasing HPAM concentration from 100 to

1000 wppm. All the HPAM solutions suffered from

mechanical degradation and loss of DR efficiency over the

shearing period. Results indicated that the resistance to

shear degradation increased with increasing polymer con-

centration. DR efficiency of 600 wppm xanthan gum (XG)

was 38%, indicating that XG was not as good a drag

reducer as HPAM. But with only 6% DR decline, XG

solution exhibited a better shear stability compared to

HPAM solutions. Mixed HPAM/XG solutions initially

exhibited greater DR (40% and 55%) compared to XG, but

due to shear degradation, DR% dropped for HPAM/XG

solutions. Compared to 200 wppm HPAM solution, addi-

tion of XG did not improve the drag reduction efficiency of

HPAM/XG mixed solutions though XG slightly improved

the resistance against mechanical degradation in HPAM/

XG mixed polymer solutions.

1 Introduction

tion from unconventional resources such as shale forma-

tions has played an important role in supplying energy in

the USA (Larch et al. 2012; Palisch et al. 2010). Reaching

economic rates of hydrocarbon production from shale

formations is only possible when micro-fractures are cre-

ated and connected through effective stimulation treat-

ments such as horizontal fracturing in multiple stages

(Loveless et al. 2014; Barati and Liang 2014; Wu et al.

2013).

pumping fracturing fluids into the wellbore at elevated flow

rates and pressures. The viscosity of a fracturing fluid has a

remarkable effect on the fracture initiation and the final

size of the fracture (Kalgaonkar and Patil 2012). The main

component of low-viscosity fracturing fluids is water and

low concentrations of polymer ranging from 0.25 to 10 lb

per thousand gallons (Bunger et al. 2013; Palisch et al.

2010). In the last decade, an amazing shift from traditional

gel-based fracturing fluids toward using slickwater has

occurred. Because of the relatively low viscosity of slick-

water, cleanup problems and damage associated with using

viscous fluids are minimized, which makes slickwater

suitable for fracturing low-permeability reservoirs (Wu

et al. 2013; Palisch et al. 2010). As a result of lower vis-

cosity, slickwater cannot suspend and transport proppants

as effectively as gelled fluids. To overcome poor proppant

transport, higher pumping rates are applied, which in turn

Edited by Xiu-Qin Zhu.

Stillwater, OK 74078, USA

DOI 10.1007/s12182-017-0152-7

et al. 2008). In order to lower the surface pumping pres-

sures and compensate for the energy losses during pump-

ing, a small amount of high molecular weight polymer is

dissolved in the fluid, which acts as a drag reducer. In

slickwater treatments, friction reducer is a significant

component of the fluid. Long, flexible chain polyacry-

lamide-based polymers are known to be the most effective

drag reduction polymers (Kim et al. 1998).

When a polymer solution is subjected to turbulent flow,

the large molecules present in the solution undergo different

conformational changes such as flow orientation, stretching,

and relaxation. These conformational changes alter the flow

field and dynamics of turbulent structures in the vicinity of

pipe wall. In the macroscopic scale, those variations result

in large drag reduction. However, mechanical degradation

of polymer solutions complicates their use (Campolo et al.

2015; Moussa and Tiu 1994). Several theories have been

proposed to explain mechanical degradation of polymer

solutions, among which extreme stretching of polymer

chains and scission of the polymer chain have been most

accepted (Rodriguez and Winding 1959). Another study

reports that chain scission occurs near the midpoint of the

polymer which is caused by the extensional features of the

turbulent flow (Lim et al. 2003; Merrill and Horn 1984).

Due to the susceptibility of PAM molecules to shear

degradation under turbulent flow conditions, researchers

have considered other candidates such as rigid polysac-

charide molecules to improve the shear stability of drag

reducers. Kim et al. used a rotating disk apparatus to verify

the DR behavior of 100 wppm XG solutions with four

different molecular weights. They observed that XG is more

resistant to shear forces than most flexible polymers (Kim

et al. 1998). Other researchers compared solutions of

polyethylene oxide (PEO), PAM, XG, and guar gum (GG).

They observed that synthetic polymers initially induced

greater DR efficiency, but as result of mechanical degra-

dation, DR efficiency of synthetic polymers declined more

quickly than the polysaccharides. The available data in the

literature suggest that XG is shear resistant at turbulent flow

conditions, but DR induced by XG is small compared to

synthetic polymers such as PAM (Soares et al. 2015; Kul-

matova 2013; Wyatt et al. 2011; Kenis 1971). According to

the literature, binary solutions of polymers can give rise to

DR efficiency and shear stability. Dingilian and Rucken-

stein (1974) investigated the DR behavior of PAM, PEO,

and carboxymethylcellulose (CMC) single and binary

solutions. They observed negative deviation from additivity

for binary solutions of two flexible polymer molecules

(PEO/PAM) and positive deviation for PAM/CMC and

PEO/CMC binary solutions, where flexible and rigid

molecules coexist in the solution. Dschagarowa and

Bochossian (1978) also observed synergism in the DR

behavior of poly-isobutylene and l,4-cis-isoprene rubber

binary solutions. They also concluded that flow conditions

can affect the degree of deviation from additivity. Malhotra

et al. (1988) verified DR of PAM/GG, GG/XG, and PAM/

XG binary solutions and concluded that the degree of DR

and synergism depend on polymer concentration and flow

rate. They also concluded that positive deviation in addi-

tivity occurs when both polymers are rigid. But, they

mentioned that their conclusions are limited to their

experimental conditions and synergism might be observed

in many other binary mixtures at higher concentrations.

Reddy and Singh (1985) verified the same binary solutions

at higher concentrations (C[ 200 wppm) and in a larger

experimental setup. Contrary to previous authors, they

observed negative deviation for PAM/polysaccharide bin-

ary solutions. They also verified the shear stability of the

polymer solutions and concluded that the solutions showing

synergism in DR produce better shear stability (Reddy and

Singh 1985). Recently Sandoval and Soares (2016) verified

the DR behavior of PAM/XG and PEO/XG binary solutions

in a pressure-driven flow loop. The authors reported clear

synergism between polymers. They concluded that the

improvement observed in the mixed solutions was related to

the change in the polymeric conformation from coiled to

elongated (Sandoval and Soares 2016). Regarding the DR

behavior of binary polymer solutions, very limited work is

reported in the literature. On the other hand, the existing

published research is limited to certain conditions such as

small-scale experimental setups (capillary tube), low flow

rates and Reynolds numbers, and certain concentrations or

molecular weights. Also, some of the available data con-

tradict each other. As mentioned above, Reddy and Singh

(1985) had a different observation from Sandoval and

Soares (2016) regarding the DR behavior of PAM/XG

binary solution, which we believe arises from the differ-

ences in the experimental setup and the molecular weights

of the polymers.

In this work, we focus on studying the DR behavior and

shear stability of anionic HPAM/XG binary polymer

solution. Anionic PAM is the partially hydrolyzed form of

polyacrylamide with more flexibility and relatively large

molar mass. Both polymers are widely used in industrial

applications such as slickwater treatments. There has been

little or no work regarding the DR behavior of anionic

HPAM and XG mixtures. We believe that it would be

interesting to verify the DR behavior of two negatively

charged molecules coexisting in a solution. Since various

HPAM and XG molecules with different molecular weights

are available in the market, we also study the behavior of

single polymer solutions, so that we can compare them

with binary solutions and assess the degree of improvement

in shear stability.

123

XG as a semirigid polymer were chosen for this investi-

gation. The molecular weights provided for PAM (Kemira

Co.) and XG (PFP Technology) by the vendors are (6–

8) 9 106 kg mol-1 and (4–5) 9 106 kg mol-1, respec-

tively. The accurate values for molar mass were measured

using light scattering (for HPAM) and viscometry (for XG)

methods. In the light scattering experiments, all solvents

were filtered through 0.02 lm cellulose acetate Millipore

filters. The HPAM solutions were prepared by dissolution

of a known amount of polymer in the 0.5 mol L-1 NaCl

solvent. The solutions were filtered through a 0.45 lm cellulose acetate Millipore filters. A concentration range of

the polymer solutions (0.2–2.0 g L-1) were analyzed using

the batch mode (without size separation) of a multi-angle

light scattering (MALS) detector (DAWN-HELEOS II,

Wyatt Technology) with a laser wavelength of 658 nm.

The specific refractive index increments (dn/dc) value of

the HPAM in 0.5 mol L-1 NaCl solution, which was

determined by an OPTILAB T-reX differential refrac-

tometer (Wyatt Technology) at 633 nm and 25 C, was 0.162 mL/g. Viscosity averaged molecular weight of XG

was measured using the method described in the literature

(Sohn et al. 2001). In this method, the intrinsic viscosity [g] was measured with an Ubbelohde capillary viscometer

(diameter capillary 0.46 mm, Schott-Gerate), immersed in

a water bath maintained at 25.0 ± 0.1 C. First, the

specific viscosity gsp was calculated from the relative vis-

cosity, which is the ratio of the viscosity of xanthan gum

solution at a certain concentration to that of the solvent.

Each concentration was measured five times. The plot of

gsp/C versus C (C is the concentration of solutions) gave a

straight line, the intercept of which was [g]. Then, using the Mark–Houwink equation the molar mass was calculated:

g½ ¼ lim c!0

gsp c

1:35 ½mL/g ð1Þ

The measured values for the molecular weights of the

polymers, HPAM and XG, were 7.2 9 106 kg mol-1 and

3.9 9 106 kg mol-1, respectively.

To establish a baseline for further studies, deionized

water was used throughout. Using an analytical balance,

polymer powders were weighed with an accuracy of

±1 mg (Mettler Toledo XS603s). The preparation of the

polymer solutions took place in a separate tank. First, the

polymer powders were gradually sprinkled into the solvent

and slowly agitated at 30 rpm, in order to prevent particles

from clumping on the surface. Then the prepared solutions

were stored overnight for complete hydration. The studied

concentrations of HPAM solutions were 100, 150, 200,

500, and 1000 wppm. In order to investigate the effect of

XG, mixed polymer solutions of 100 wppm

HPAM ? 100 wppm XG (total C = 200 wppm), 150

wppm HPAM ? 100 wppm XG (total C = 250 wppm),

and for comparison, 600 wppm XG solutions were

prepared.

A closed-loop flow system was used for drag reduction and

turbulent flow measurements (Fig. 1). The system is

comprised of a 60-L supply tank connected to a progressive

cavity pump (SEEPEX BN 10-12) with a pumping capacity

of 30 GPM (113.56 L/min), and a seamless stainless steel

horizontal pipe test section of L = 8 ft. (2.44 m) and inner

diameter of 1 in. (2.54 cm). The flow rate of the system

was measured using a mass flow meter (OPTIMASS 1000,

KROHNE) with an accuracy of ±0.15% and a repeatability

of ±0.05% as stated by the manufacturer. The pressure

drop data along the measuring length of the pipe were

gathered using a membrane differential pressure transducer

(PX409, OMEGA). At each flow rate, the Fanning friction

factor is calculated by:

ð2Þ

Here, f is the Fanning friction factor, q is the fluid density,

U is the average velocity, DP is pressure drop in the

measurement length of L, and D is the internal diameter of

the pipe.

the polymer solutions was defined as:

DR ¼ fw fs

where subscripts ‘‘w’’ and ‘‘s’’ stand for water and polymer

solution, respectively, and ‘‘Re = const.’’ signifies the fact

that the comparison between the flows is made at the same

Reynolds numbers. Here Re = qUD/ga, and ga is fluid

viscosity. In drag reduction experiments, the flow rate was

increased stepwise (and kept constant for 1 min at each

flow rate), and then, the polymer solutions were sheared in

the flow loop at maximum flow of 30 GPM for 2 h and

sampling was performed eight times at shearing periods of

t = 0, 15, 30, 45, 60, 80, 100, and 120 min. After the

shearing process, the flow rate was decreased stepwise in

the same manner as it was increased.

Viscosity measurements were carried out in a DHR

controlled stress rheometer. The instrument is equipped

with a Peltier system to control sample temperature. In our

experiments, sample temperature was maintained at

25 ± 0.01 C. The geometry used in the apparent viscosity

414 Pet. Sci. (2017) 14:412–423

123

angle were 60 mm and 2, respectively. Approximately,

2 mL of the solution was placed between the cone (rotating

plate) and the fixed plate and the instrument was set to the

strain control mode. In this mode, shear rate ( _c) was log-

arithmically increased from 0.01 to 1000 s-1 and shear

stress was measured simultaneously, and then, apparent

viscosity was calculated using ga ¼ r= _c correlation, where r and ga are shear stress and apparent viscosity, respec-

tively. The power-law and Carreau–Yasuda viscosity

models were used for fitting the viscosity data.

In the power-law model, n (behavior index) is a measure

of deviation from Newtonian behavior and K (consistency

index) is a measure of average viscosity. K and n known as

power-law parameters were used in friction factor

calculations.

ga ¼ Kð _cÞn1 ð4Þ g g1 g0 g1

¼ 1þ ðk _cÞa½ n1 a ð5Þ

In the Carreau–Yasuda equation, g is the shear viscosity, and g0 and g? are viscosities at zero-shear and infinite-

shear plateaus, while k, n, and a represent the inverse shear

rate at the onset of shear thinning, power-law index, and

transition index, respectively.

3.1 Polyacrylamide solutions

In order to assess the degree of drag reduction and polymer

degradation, several samples were taken at specified

intervals over the shearing process. Shear stress and

apparent viscosity of the samples were measured in the

rheometer, and the power-law and Carreau–Yasuda

parameters were calculated. For Newtonian fluids, the

value of n is 1 and for shear-thinning fluids, such as

polymer solutions, n is\1. As the value of n deviates from

1, the degree of non-Newtonian behavior increased. The

Carreau–Yasuda and power-law parameters calculated for

different concentrations of the anionic polyacrylamide are

shown in Table 1 and Fig. 2a, b, respectively. Comparison

of power-law parameters of fresh (zero shearing time)

HPAM solutions showed that by increasing concentration,

values of K increased and n values decreased, indicating

increased non-Newtonian behavior. It can also be found

that, as the shearing time increased, the values of power-

law parameters changed for all the polymer solutions.

Figure 2a shows that, over the shearing time, K values of

HPAM solutions decreased and n values increased and get

close to one (Newtonian behavior). The difference in the

n values of the solutions before and after the shearing was

P

Data acquisition and control

Fig. 1 Schematic illustration of the flow loop; instrumentation consists of a digital flow meter (F), differential pressure transducer (P), valves

(V), and temperature sensors (T)

Pet. Sci. (2017) 14:412–423 415

123

overall change in n values (after the shearing period) was

35% for a 100 wppm solution, and by increasing concen-

tration, the maximum change in n values (152%) appeared

at 200 wppm. As the concentration increased above

200 wppm, n droped to 69% for the 1000 wppm solution.

As a result of shear degradation and consequently viscosity

reduction, K values declined. By increasing concentration

from 100 wppm to 1000 wppm, K values reached a max-

imum decline of 64% at 200 wppm, but with further con-

centration increase a 33% decline in K value was found for

1000 wppm HPAM solution.

Fig. 3, where the apparent viscosity of the 200 wppm

HPAM solution, at shear rates under 10 s-1, undergoes

drastic reduction as the circulation time increases. The

reason that we only saw changes at lower shear rates might

be related to the scission of the molecules that belong to the

high tale of the molecular weight distribution of the

polymer (Liberatore et al. 2004). Those molecules con-

tributed to the formation of the zero-shear viscosity

plateau.

Prandtl–Karman coordinates are a semilog graph of f -

versus Re.f, where f and Re are Fanning friction factor and

Reynolds number, respectively. Using Prandtl–Karman

Table 1 Parameters of

Carreau–Yasuda model for

HPAM, XG, and HPAM/XG

solutions

Concentration of solution g0, Pa s g?, Pa s k, s a n

100 wppm HPAM 0.0835 0.0035 4.96 1.37 0.37

150 wppm HPAM 0.2668 0.0041 5.46 3.15 0.26

200 wppm HPAM 0.3717 0.0042 5.80 3.14 0.27

500 wppm HPAM 1.2105 0.0052 8.70 3.74 0.26

1000 wppm HPAM 3.5071 0.0067 10.1 3.52 0.21

600 wppm XG 0.2689 0.0040 5.34 1.92 0.43

100 wppm HPAM ? 100 wppm XG 0.1331 0.0039 4.18 2.51 0.36

150 wppm HPAM ? 100 wppm XG 0.2873 0.0038 7.2 2.28 0.33

0

0.1

0.2

0.3

0.4

0.5

0.6

0.7

0.8

0.9

P ow

er -la

w in

de x

100 wppm

150 wppm

200 wppm

500 wppm

1000 wppm

Time, min

K , P

a· sn

Time, min

Fig. 2 Power-law model parameters variation over shearing time for HPAM solutions

1

10

100

1000

0.01 0.1 1 10 100 1000

Sample 1 Sample 2 Sample 3 Sample 4 Sample 5 Sample 6 Sample 7 Sample 8

η a , m

Fig. 3 Apparent viscosity of 200 wppm sheared HPAM samples

(samples 1–8: fresh, 15, 30, 45, 60, 80, 100, and 120 min shearing

time)

123

coordinates, the degree of DR of polymer solutions can be

compared with respect to the boundaries of drag reduction;

the onset of drag reduction as the point of departure from

Prandtl–Karman law and maximum drag reduction (MDR)

or Virk’s asymptote (White and Mungal 2008; Virk 1975).

Prandtl–Karman plot for different concentrations of HPAM

is shown in Fig. 4. Three flow regimes can be detected:

(a) Re ffiffiffi f

obey Poiseuille’s law.

p \350; laminar to turbulent transition.

(c) Re ffiffiffi f

p [ 350; turbulent flow.

It is observed that except for the laminar to turbulent

transition region, the turbulent friction factor data for the

solutions are bounded in the area between the two universal

asymptotes and the data points are linear for all

concentrations.

Results of linear fitting of the data points in the turbulent

region (Table 2) revealed that by increasing the concen-

tration of polymer, the slope of the lines tended to increase.

According to the literature, the slope increment with

respect to the Prandtl–Karman law (d) is proportional to the

square root of polymer concentration (d / ffiffiffiffi C

p ) with a

values are reported in Table 2. The proportionality constant

for the HPAM used in this work is calculated to be

0.27 ± 0.05. Figure 4 shows that by increasing HPAM

concentration, the extent of DR increases and the data

points approach Virk’s asymptote. Among different con-

centrations, the extent of DR and slope of data points for

100 wppm HPAM solution were closest to the Prandtl–

Karman line (the onset of DR). On the other hand, the

greatest DR belongs to the 1000 wppm solution. For

solutions with polymer content greater than 200 wppm, in

200\Re ffiffiffi f

p \500 range, the data points were nearly tan-

gential to the MDR line, but by increasing the flow rates

(Reynolds number), the data points tended to deviate from

MDR. Results indicated that further increase in concen-

tration did not have a large effect on the degree of DR in

the experimental conditions of this work.

The effect of polymer concentration and mechanical

degradation on the Fanning friction factor of HPAM

solutions is shown in Fig. 5a, b, respectively. It can be seen

that even at low concentrations of polymer (100 wppm),

Fanning friction factor values were much lower than those

of water. Increasing polymer concentration resulted in

further reduction in friction factors (data points get close to

the maximum drag reduction asymptote), and conse-

quently, drag reduction efficiency increased. The smallest

values of friction factors at different Reynolds numbers

belong to 1000 wppm solution. It was also observed that

the difference between turbulent friction factors of 200,

500, and 1000 wppm solutions was very small, which is in

agreement with the results shown in Prandtl–Karman

coordinates, indicating that at the studied range of Rey-

nolds numbers, DR efficiency was close to its maximum

value (MDR); further increase in concentration did not

change friction factors. We can also observe that as the

Reynolds numbers increased, the data points tended to

deviate from MDR.

Shearing had a large impact on reducing the DR ability

of polyacrylamide solutions. Comparing the friction factors

of 200 wppm HPAM solution at different Reynolds num-

bers (Fig. 5b) showed a 30%–50% decline after 2 h of

shearing. It can be observed that as a result of shearing,

friction factor values moved away from MDR line and

shifted toward water friction factors at different Reynolds

numbers. Although flow rate was constant for all the

experiments, a shift in the data points of the sheared

samples toward lower Reynolds numbers was observed.

0

5

10

15

20

25

100 wppm-Fresh 150 wppm-Fresh 200 wppm-Fresh 500 wppm-Fresh 1000 wppm-Fresh

Poiseuille’s law

Fig. 4 Prandtl–Karman coordinates for HPAM solutions

Table 2 Linear fit results of

turbulent regime Concentration, wppm Linear fit equation R2 Slope increment (d)

100 1= ffiffiffi f

p ¼ 6:0 logRe

123

The shift was an indication of alteration in the flow regime,

which occurred due to the change in the rheological

properties of the solutions as a result of shear degradation.

Figure 6 shows the changes in the DR% over shearing time

for different concentrations of HPAM at constant flow rate.

It was observed that, for fresh samples (t = 0), the extent

of DR increased from 30% to 67% by increasing polymer

concentration from 100 to 1000 wppm. Results also indi-

cated that solutions above 200 wppm produced nearly

identical DR at the early stages of shearing (t\ 20 min),

which corresponds to the results shown in Prandtl–Karman

coordinates (Fig. 4). But beyond 20 min, the DR curves

tended to diverge, indicating that the degree of shear

degradation was different for each polymer concentration.

Ptasinski et al. (2003) reported that in flexible polymers

such as HPAM, as shear force reached a certain level, the

molecules stretch and consequently effective viscosity

increased, the turbulent buffer layer thickened, and due to

dissipation of the energy from turbulent fluctuations drag

was reduced. It is also known that drag is reduced when

turbulent flow interacts with polymer networks. When

polymer concentration is high enough (above critical

overlap concentration, C*), polymer chains are packed

closer and begin to interact with each other and form

entangled networks (Skelland and Meng 1996).

The decline in the degree of DR was observed at all the

concentrations of HPAM solution. Resistance to mechani-

cal degradation over the shearing period is shown in Fig. 7.

Results showed that, as the concentration increased, the

resistance to mechanical degradation also increased. This

made the 100 wppm solution the least resistant and

1000 wppm solution the most resistant to mechanical

degradation. These results agreed with those reported by as

Soares et al. (2015), indicating that increasing polymer

concentration (PAM or PEO) in the solution could increase

the resistance to mechanical degradation. It was also

observed that the shear stabilities of 100, 150, 200 wppm

solutions were very close and followed the same trends. In

other words, 200 ppm solution was only slightly more

resistant to degradation (DRt=120/DRmax = 0.5) than

Fr ic

tio n

fa ct

0.1(a) (b)

Fig. 5 Friction factor versus Re: a effect of HPAM concentration and b effect of shearing on 200 wppm HPAM

0

10

20

30

40

50

60

70

80

% D

100 wppm 150 wppm 200 wppm 500 wppm 1000 wppm

MDR

Fig. 6 %Drag reduction for different concentrations of HPAM at

30 GPM (113.56 L/min)

123

100 wppm solution (DRt=120/DRmax = 0.39). But, above

200 wppm a sudden rise in the shear resistance of the

solutions was observed. Both 500 and 1000 wppm solu-

tions showed superior shear stability compared to other

solutions. We found that although 200 wppm HPAM

solution had similar initial DR% to 500 and 1000 wppm

solutions (Fig. 6), it had a larger decline in DR (Fig. 7).

The values of DRt=120/DRmax for 500 and 1000 wppm

solutions were 0.62 and 0.72 at the end of 2-h shearing

period, respectively. It is also interesting to note that the

DR/DRmax declined at a slower rate after t = 60 min. For

example, the reduction in DR/DRmax value for 1000 wppm

solution from t = 60 min to t = 120 min was only 0.06.

From viscosity measurements, the critical overlap con-

centration (the concentration that marks the beginning of

polymer–polymer interaction) of the HPAM solution was

determined to be 200 wppm. At C\ 200 wppm, there was

no polymer network, so there was no decline due to

polymer network breakup, but at C[ 200 wppm, the net-

works were more entangled and upon deformation can

recover quickly. Also, it seems that at higher concentra-

tions (C[ 200 wppm), the extensional force from the

turbulent flow was distributed among a larger number of

molecules, which resulted in a lower number of chain

scissions and higher DR stability. But at C\ 200 wppm

polymer networks just began to form and were weak.

Therefore, at the beginning of the shearing process DR

efficiency increased, but gradually as shear forces acted,

unstable polymer networks, as well as individual polymer

molecules broke up, which resulted in a large decline in the

DR efficiency of C\ 200 wppm HPAM solutions com-

pared to higher concentrations.

Another result was that the rate of DR decline was fast

in the first 60–80 min of the shearing process. This is

probably due to the presence of longer chains of polymer in

the fresh solutions, which are more susceptible to chain

scissions (require less energy to break). After 60 min, the

gap between DR lines (Fig. 6) remained nearly constant,

which indicated that polymer chains were broken up at a

similar rate at all the concentrations.

Several models for correlating the DR behavior of

polymer solutions can be found in the literature. Two of the

most common models are the exponential decay model

(Bello et al. 1996) and Brostow’s model (Brostow 1983).

Based on the exponential decay model proposed by Bello

et al. (1996), DR follows an exponential decline with time

for polyacrylamide and polysaccharide solutions:

DR% tð Þ=DR% 0ð Þ ¼ e t=kð Þ ð6Þ

where DR% (t) and DR% (0) (or DRmax) are percent drag

reduction at times t and t = 0, respectively, and k is an

adjustable parameter. Brostow’s equation is a more general

model, which has been applied to various shear degradation

applications (Lim et al. 2003) and has been developed to

quantitatively describe DR and its changes with time:

DR% tð Þ=DR% 0ð Þ ¼ ½1þWð1 e htð ÞÞ1 ð7Þ

Here W is the average number of vulnerability points per

chain and h is called rate constant.

The two models were used in this work to correlate the

DR data of HPAM and HPAM/XG solutions. Calculated

model parameters and goodness of fit (R2) for both models

are reported in Table 3. The solid lines in Fig. 6 represent

the fitting results. It can be found that for the studied

concentrations of HPAM solution, both models describe

the degradation behavior well, though Brostow’s model

gives better fits and its predicted values are more accurate.

0

0.1

0.2

0.3

0.4

0.5

0.6

0.7

0.8

0.9

1.0

100 wppm 150 wppm 200 wppm 500 wppm 1000 wppm

Time, min

D R

/D R

m ax

solutions at 30 GPM (113.56 L/min)

Table 3 Parameters of Brostow

and exponential decay models

k, min R2 W h, min-1 R2

100 87.32 0.96 374.2 32.7e-5 0.94

150 146.7 0.97 43.43 2.3e-4 0.98

200 162.3 0.95 2.723 3.9e-3 0.99

500 245.0 0.90 0.8628 9.6e-3 0.98

1000 312.1 0.88 0.6351 8.1e-3 0.96

Pet. Sci. (2017) 14:412–423 419

123

In order to verify the possibility of stabilizing HPAM with

XG, mixed solutions were prepared and sheared in the

same manner as the HPAM solutions. Based on the results

obtained from the previous section, the DR behavior of

binary polymer solutions was compared to that of

200 wppm HPAM solution. Several authors have men-

tioned that the degree of DR in XG solutions depends on

the concentration and molar mass of XG (Soares et al.

2015; Pereira et al. 2013). So higher concentrations of XG

are required to reach the same level of DR as HPAM. Our

preliminary experiments showed that the DR efficiency of

600 wppm XG was close to the DR values of 200 wppm

HPAM.

solutions and solutions of 600 wppm XG and 200 wppm

HPAM are shown in Fig. 8a. It was found that, although

polymer concentration in the 600 wppm XG solution was

greater than that of 200 wppm HPAM solution, the

600 wppm XG solution possessed greater friction factors.

Higher flexibility of HPAM polymer chains with respect to

semirigid XG chains resulted in higher energy adsorption

(stretching) due to interaction with dynamic turbulent flow

and subsequently, superior drag reduction capability of

flexible polymers. Also, it was found that in the fresh

binary solutions, there is no outstanding synergetic effect

between HPAM and XG molecules. Even the 150 wppm

HPAM ? 100 wppm XG solution, which has a higher total

polymer concentration, showed larger friction factors than

200 wppm HPAM.

after 120 min of shearing. Because of high shear stability,

XG solution maintained its initial friction reduction

0.001

0.01

0.1

0.003

0.03

(a)

(b)

Fig. 8 Fanning friction factor of mixed solutions in a fresh form and b after shearing for 120 min

420 Pet. Sci. (2017) 14:412–423

123

efficiency, with a relatively small change in friction factor

values. But for the mixed HPAM/XG solutions, the friction

factor values largely increased as a result of shearing. It is

interesting to note that 200 wppm HPAM solution had a

larger increase in its friction factors than mixed solutions

(Fig. 8b). This suggested that addition of XG was benefi-

cial in controlling the shear degradation of HPAM. The

decline in the DR efficiency and shear resistance of the

samples over shearing time is shown in Figs. 9 and 10.

Also, as mentioned above, Brostow’s and exponential

decay models were used to correlate DR with time (solid

lines in Fig. 9; Table 4).

The results indicated that the DR efficiencies of both

HPAM and XG binary solutions were smaller than that of

200 wppm HPAM solution, indicating that partially

replacing HPAM with XG in the binary solutions had

reduced the DR efficiency of the single HPAM solution.

Regarding the DR behavior of HPAM/XG binary mixtures,

different views can be found in the literature. Sandoval and

Soares (2016) recently reported that the DR efficiency of

HPAM/XG mixture is close to the DR values of the single

HPAM solution at the same total concentration. However,

they confirmed that the synergetic effect in PAM/XG

mixture is not as notable as PEO/XG. Reddy and Singh

(1985) also studied PAM/XG mixtures and reported that

the single PAM solution has a higher DR efficiency than a

binary mixture. Their data were limited to fresh solutions.

We believe that the differences in the reported data might

be attributed to the differences in the experimental condi-

tions. In our work, since we were dealing with two nega-

tively charged polymers in the solution, we would expect

to obtain different results. We also believed that due to the

higher flexibility (higher molecular weight) of the anionic

HPAM used in our experiments, HPAM molecules were

more susceptible to scission and the interaction between

HPAM and XG was reduced. Compared to 600 wppm XG

solution, the DR% of 100 wppm HPAM/150 wppm XG

solution was high only in the first 60 min of the shearing

process and after that, as a result of mechanical degradation

the DR values declined. Also, it was found that the

100 wppm HPAM/100 wppm XG solution was less effi-

cient in DR than the 600 wppm XG solution from the

beginning till end of the shearing period. Comparison of

the shear resistance (DR/DRmax) of the solutions revealed

that, as expected, 600 wppm XG solution had the best

shear stability among all the solutions and the least decline

in DR over the shearing period (0.15 decline in DR/DRmax

value). Contrary to XG, 200 wppm HPAM and the binary

HPAM/XG solutions suffered from poor shear resistance

and a large decline in their DR efficiencies. These results

are in agreement with the results reported by Sandoval and

Soares (2016). It is interesting to note that the shear

resistance of both binary solutions and 200 wppm HPAM

solution was nearly identical.

% D

n

Time, min 200 wppm HPAM 600 wppm XG 100 wppm HPAM + 100 wppm XG 150 wppm HPAM+100 wppm XG

MDR

Fig. 9 %Drag reduction for mixed HPAM/XG solutions at 30 GPM

(113.56 L/min)

% D

n

Time, min 200 wppm HPAM 600 wppm XG 100 wppm HPAM + 100 wppm XG 150 wppm HPAM+100 wppm XG

Fig. 10 Effect of shearing on DR decline for mixed HPAM/XG

solutions

and exponential decay models

for mixed HPAM/XG solutions

k, min R2 W h, min-1 R2

200 (HPAM) 145 0.92 1.792 6.8e-3 0.99

600 (XG) 571 0.94 0.3853 8.8e-3 0.96

100 (HPAM) ? 100 (XG) 137 0.92 44.49 2.2e-4 0.96

150 (HPAM) ? 100 (XG) 127 0.89 1.768 8.4e-3 0.99

Pet. Sci. (2017) 14:412–423 421

123

inferred that addition of XG reduced the DR capability of

mixed solutions (DR% = 40% and 55%) with respect to

200 wppm HPAM solution. Also results suggested that

increasing HPAM concentration in the mixed solutions

does not change the DR efficiency decline significantly.

Since there was only a small amount of chain degradation

in semirigid polymers, the extent of DR depended only on

the interaction between polymer chains and entanglements,

which is directly related to polymer concentration. It

should be considered that the concentration of XG was

100 wppm for mixed solutions, which is below the critical

concentration of XG (C* & 300 ppm). Hence, as sug-

gested by other authors (Wyatt et al. 2011; Berman 1978),

mixing HPAM with higher concentrations of XG would be

more beneficial in maintaining high DR efficiency and

even better control of shear degradation of polyacrylamide

solutions, which is the subject of our future work. Same as

for the HPAM solutions, Brostow and exponential decay

models were used to correlate the drag reduction behavior

over time for the HPAM/XG mixed solutions. The result is

shown in Fig. 9 and Table 4. It can be found that both

models give good fitting, but similar to HPAM solutions,

the Brostow’s model correlated the DR reduction data

better.

concentrations of HPAM, 1000 wppm solution has the

highest drag reduction efficiency and the lowest decline in

DR%. Increasing the concentration above 200 wppm does

not change the DR% of the fresh samples significantly,

though increasing concentration increases resistance to

mechanical degradation. Results also indicate that mixing

flexible HPAM with XG did not improve the degree of DR

significantly, but slightly improved the DR stability of

HPAM solutions. Since the drag reduction of rigid poly-

mers depends only on concentration, mixing HPAM with

higher concentrations of XG might be beneficial in main-

taining the DR efficiency of HPAM as well as improving

its shear stability. Brostow and exponential decay models

were used to correlate the drag reduction decline data.

Results indicate that both models can correlate the DR

behavior of HPAM, as well as mixed HPAM/XG solutions.

Brostow’s model gave slightly better fits.

Acknowledgements The authors would like to thank the Research

Partnership to Secure Energy for America (RPSEA) and Oklahoma

State University Chemical Engineering Department for partial support

of this project.

Open Access This article is distributed under the terms of the

Creative Commons Attribution 4.0 International License (http://crea

tivecommons.org/licenses/by/4.0/), which permits unrestricted use,

distribution, and reproduction in any medium, provided you give

appropriate credit to the original author(s) and the source, provide a

link to the Creative Commons license, and indicate if changes were

made.

References

Barati R, Liang J-T. A review of fracturing fluid systems used for

hydraulic fracturing of oil and gas wells. J Appl Polym Sci.

2014;131(16). doi:10.1002/app.40735.

Bello JB, Muller AJ, Saez AE. Effect of intermolecular cross links on

drag reduction by polymer solutions. Polym Bull.

1996;36(1):111–8. doi:10.1007/BF00296015.

Berman NS. Drag reduction by polymers. Annu Rev Fluid Mech.

1978;10(1):47–64.

solutions in flow. Polymer. 1983;24(5):631–8.

Bunger AP, McLennan J, Jeffrey R. Effective and sustainable

hydraulic fracturing. InTech, Janeza Trdine. 2013;9:51000.

Campolo M, Simeoni M, Lapasin R, Soldati A. Turbulent drag

reduction by biopolymers in large scale pipes. J Fluids Eng.

2015;137(4):041102.

AIChE J. 1974;20(6):1222–4.

Rheol Acta. 1978;17(4):426–32.

crosslinked fracturing fluids. 1 January 2012. SPE: Society of

Petroleum Engineers; 2012.

Kaufman PB, Penny GS, Paktinat J. Critical evaluation of additives

used in shale slickwater fracs. 1 January 2008. SPE: Society of

Petroleum Engineers; 2008.

hydrodynamic degradation of polysaccharides and synthetic

polymers. J Appl Polym Sci. 1971;15(3):607–18.

Kim CA, Choi HJ, Kim CB, Jhon MS. Drag reduction characteristics

of polysaccharide xanthan gum. Macromol Rapid Commun.

1998;19(8):419–22. doi:10.1002/(SICI)1521-

3927(19980801)19:8\419:AID-MARC419[3.0.CO;2-0.

Kulmatova D. Turbulent drag reduction by additives. Phys Rev Lett.

2013;84:4765–8.

Larch KL, Aminian K, Ameri S. The impact of multistage fracturing

on the production performance of the horizontal wells in shale

formations. 1 January 2012. SPE: Society of Petroleum Engi-

neers; 2012.

Liberatore MW, Baik S, McHugh AJ, Hanratty TJ. Turbulent drag

reduction of polyacrylamide solutions: effect of degradation on

molecular weight distribution. J Nonnewton Fluid Mech.

2004;123(2):175–83.

Lim S, Choi H, Lee S, So J, Chan C. k-DNA induced turbulent drag

reduction and its characteristics. Macromolecules.

2003;36(14):5348–54.

Loveless D, Holtsclaw J, Weaver JD, Ogle JW, Saini RK.

Multifunctional boronic acid crosslinker for fracturing fluids.

19 January 2014. IPTC: International Petroleum Technology

Conference; 2014.

Malhotra J, Chaturvedi P, Singh R. Drag reduction by polymer–

polymer mixtures. J Appl Polym Sci. 1988;36(4):837–58.

422 Pet. Sci. (2017) 14:412–423

extensional and turbulent flows. Polym Commun. 1984;25(5):

144–6.

Moussa T, Tiu C. Factors affecting polymer degradation in turbulent

pipe flow. Chem Eng Sci. 1994;49(10):1681–92.

Palisch TT, Vincent M, Handren PJ. Slickwater fracturing: food for

thought. SPE Prod Oper. 2010;. doi:10.2118/115766-PA.

Pereira AS, Andrade RM, Soares EJ. Drag reduction induced by

flexible and rigid molecules in a turbulent flow into a rotating

cylindrical double gap device: comparison between Poly

(ethylene oxide), Polyacrylamide, and Xanthan Gum. J Nonnew-

ton Fluid Mech. 2013;202:72–87. doi:10.1016/j.jnnfm.2013.09.

008.

Ptasinski P, Boersma B, Nieuwstadt F, Hulsen M, Van den Brule B,

Hunt J. Turbulent channel flow near maximum drag reduction:

simulations, experiments and mechanisms. J Fluid Mech.

2003;490:251–91.

Reddy G, Singh R. Drag reduction effectiveness and shear stability of

polymer–polymer and polymer–fibre mixtures in recirculatory

turbulent flow of water. Rheol Acta. 1985;24(3):296–311.

Rodriguez F, Winding C. Mechanical degradation of dilute poly-

isobutylene solutions. Ind Eng Chem. 1959;51(10):1281–4.

doi:10.1021/ie50598a034.

Sandoval GA, Soares EJ. Effect of combined polymers on the loss of

efficiency caused by mechanical degradation in drag reducing

flows through straight tubes. Rheol Acta. 2016;55(7):559–569.

Skelland A, Meng X. The critical concentration at which interaction

between polymer molecules begins in dilute solutions. Polym

Plast Technol Eng. 1996;35(6):935–45.

Soares EJ, Sandoval GA, Silveira L, Pereira AS, Trevelin R, Thomaz

F. Loss of efficiency of polymeric drag reducers induced by high

Reynolds number flows in tubes with imposed pressure. Phys

Fluids (1994–present). 2015;27(12):125105.

Sohn J-I, Kim C, Choi H, Jhon M. Drag-reduction effectiveness of

xanthan gum in a rotating disk apparatus. Carbohydr Polym.

2001;45(1):61–8.

Virk P, Baher H. The effect of polymer concentration on drag

reduction. Chem Eng Sci. 1970;25(7):1183–9.

Virk PS. Drag reduction fundamentals. AIChE J. 1975;21(4):625–56.

doi:10.1002/aic.690210402.

White CM, Mungal MG. Mechanics and prediction of turbulent drag

reduction with polymer additives. Annu Rev Fluid Mech.

2008;40:235–56.

Wu Q, Sun Y, Zhang H, Ma Y, Bai B, Wei M. Experimental study of

friction reducer flows in microfracture during slickwater frac-

turing. 8 April 2013. SPE: Society of Petroleum Engineers;

2013.

ness of dilute and entangled xanthan in turbulent pipe flow.

J Nonnewton Fluid Mech. 2011;166(1–2):25–31. doi:10.1016/j.

jnnfm.2010.10.002.

Abstract

Introduction

Results and discussion

Received: 6 October 2016 / Published online: 28 March 2017

The Author(s) 2017. This article is an open access publication

Abstract Partially hydrolyzed polyacrylamide (HPAM) as

the main component of slickwater fracturing fluid is a

shear-sensitive polymer, which suffers from mechanical

degradation at turbulent flow rates. Five different concen-

trations of HPAM as well as mixtures of polyacrylamide/

xanthan gum were prepared to investigate the possibility of

improving shear stability of HPAM. Drag reduction (DR)

measurements were performed in a closed flow loop. For

HPAM solutions, the extent of DR increased from 30% to

67% with increasing HPAM concentration from 100 to

1000 wppm. All the HPAM solutions suffered from

mechanical degradation and loss of DR efficiency over the

shearing period. Results indicated that the resistance to

shear degradation increased with increasing polymer con-

centration. DR efficiency of 600 wppm xanthan gum (XG)

was 38%, indicating that XG was not as good a drag

reducer as HPAM. But with only 6% DR decline, XG

solution exhibited a better shear stability compared to

HPAM solutions. Mixed HPAM/XG solutions initially

exhibited greater DR (40% and 55%) compared to XG, but

due to shear degradation, DR% dropped for HPAM/XG

solutions. Compared to 200 wppm HPAM solution, addi-

tion of XG did not improve the drag reduction efficiency of

HPAM/XG mixed solutions though XG slightly improved

the resistance against mechanical degradation in HPAM/

XG mixed polymer solutions.

1 Introduction

tion from unconventional resources such as shale forma-

tions has played an important role in supplying energy in

the USA (Larch et al. 2012; Palisch et al. 2010). Reaching

economic rates of hydrocarbon production from shale

formations is only possible when micro-fractures are cre-

ated and connected through effective stimulation treat-

ments such as horizontal fracturing in multiple stages

(Loveless et al. 2014; Barati and Liang 2014; Wu et al.

2013).

pumping fracturing fluids into the wellbore at elevated flow

rates and pressures. The viscosity of a fracturing fluid has a

remarkable effect on the fracture initiation and the final

size of the fracture (Kalgaonkar and Patil 2012). The main

component of low-viscosity fracturing fluids is water and

low concentrations of polymer ranging from 0.25 to 10 lb

per thousand gallons (Bunger et al. 2013; Palisch et al.

2010). In the last decade, an amazing shift from traditional

gel-based fracturing fluids toward using slickwater has

occurred. Because of the relatively low viscosity of slick-

water, cleanup problems and damage associated with using

viscous fluids are minimized, which makes slickwater

suitable for fracturing low-permeability reservoirs (Wu

et al. 2013; Palisch et al. 2010). As a result of lower vis-

cosity, slickwater cannot suspend and transport proppants

as effectively as gelled fluids. To overcome poor proppant

transport, higher pumping rates are applied, which in turn

Edited by Xiu-Qin Zhu.

Stillwater, OK 74078, USA

DOI 10.1007/s12182-017-0152-7

et al. 2008). In order to lower the surface pumping pres-

sures and compensate for the energy losses during pump-

ing, a small amount of high molecular weight polymer is

dissolved in the fluid, which acts as a drag reducer. In

slickwater treatments, friction reducer is a significant

component of the fluid. Long, flexible chain polyacry-

lamide-based polymers are known to be the most effective

drag reduction polymers (Kim et al. 1998).

When a polymer solution is subjected to turbulent flow,

the large molecules present in the solution undergo different

conformational changes such as flow orientation, stretching,

and relaxation. These conformational changes alter the flow

field and dynamics of turbulent structures in the vicinity of

pipe wall. In the macroscopic scale, those variations result

in large drag reduction. However, mechanical degradation

of polymer solutions complicates their use (Campolo et al.

2015; Moussa and Tiu 1994). Several theories have been

proposed to explain mechanical degradation of polymer

solutions, among which extreme stretching of polymer

chains and scission of the polymer chain have been most

accepted (Rodriguez and Winding 1959). Another study

reports that chain scission occurs near the midpoint of the

polymer which is caused by the extensional features of the

turbulent flow (Lim et al. 2003; Merrill and Horn 1984).

Due to the susceptibility of PAM molecules to shear

degradation under turbulent flow conditions, researchers

have considered other candidates such as rigid polysac-

charide molecules to improve the shear stability of drag

reducers. Kim et al. used a rotating disk apparatus to verify

the DR behavior of 100 wppm XG solutions with four

different molecular weights. They observed that XG is more

resistant to shear forces than most flexible polymers (Kim

et al. 1998). Other researchers compared solutions of

polyethylene oxide (PEO), PAM, XG, and guar gum (GG).

They observed that synthetic polymers initially induced

greater DR efficiency, but as result of mechanical degra-

dation, DR efficiency of synthetic polymers declined more

quickly than the polysaccharides. The available data in the

literature suggest that XG is shear resistant at turbulent flow

conditions, but DR induced by XG is small compared to

synthetic polymers such as PAM (Soares et al. 2015; Kul-

matova 2013; Wyatt et al. 2011; Kenis 1971). According to

the literature, binary solutions of polymers can give rise to

DR efficiency and shear stability. Dingilian and Rucken-

stein (1974) investigated the DR behavior of PAM, PEO,

and carboxymethylcellulose (CMC) single and binary

solutions. They observed negative deviation from additivity

for binary solutions of two flexible polymer molecules

(PEO/PAM) and positive deviation for PAM/CMC and

PEO/CMC binary solutions, where flexible and rigid

molecules coexist in the solution. Dschagarowa and

Bochossian (1978) also observed synergism in the DR

behavior of poly-isobutylene and l,4-cis-isoprene rubber

binary solutions. They also concluded that flow conditions

can affect the degree of deviation from additivity. Malhotra

et al. (1988) verified DR of PAM/GG, GG/XG, and PAM/

XG binary solutions and concluded that the degree of DR

and synergism depend on polymer concentration and flow

rate. They also concluded that positive deviation in addi-

tivity occurs when both polymers are rigid. But, they

mentioned that their conclusions are limited to their

experimental conditions and synergism might be observed

in many other binary mixtures at higher concentrations.

Reddy and Singh (1985) verified the same binary solutions

at higher concentrations (C[ 200 wppm) and in a larger

experimental setup. Contrary to previous authors, they

observed negative deviation for PAM/polysaccharide bin-

ary solutions. They also verified the shear stability of the

polymer solutions and concluded that the solutions showing

synergism in DR produce better shear stability (Reddy and

Singh 1985). Recently Sandoval and Soares (2016) verified

the DR behavior of PAM/XG and PEO/XG binary solutions

in a pressure-driven flow loop. The authors reported clear

synergism between polymers. They concluded that the

improvement observed in the mixed solutions was related to

the change in the polymeric conformation from coiled to

elongated (Sandoval and Soares 2016). Regarding the DR

behavior of binary polymer solutions, very limited work is

reported in the literature. On the other hand, the existing

published research is limited to certain conditions such as

small-scale experimental setups (capillary tube), low flow

rates and Reynolds numbers, and certain concentrations or

molecular weights. Also, some of the available data con-

tradict each other. As mentioned above, Reddy and Singh

(1985) had a different observation from Sandoval and

Soares (2016) regarding the DR behavior of PAM/XG

binary solution, which we believe arises from the differ-

ences in the experimental setup and the molecular weights

of the polymers.

In this work, we focus on studying the DR behavior and

shear stability of anionic HPAM/XG binary polymer

solution. Anionic PAM is the partially hydrolyzed form of

polyacrylamide with more flexibility and relatively large

molar mass. Both polymers are widely used in industrial

applications such as slickwater treatments. There has been

little or no work regarding the DR behavior of anionic

HPAM and XG mixtures. We believe that it would be

interesting to verify the DR behavior of two negatively

charged molecules coexisting in a solution. Since various

HPAM and XG molecules with different molecular weights

are available in the market, we also study the behavior of

single polymer solutions, so that we can compare them

with binary solutions and assess the degree of improvement

in shear stability.

123

XG as a semirigid polymer were chosen for this investi-

gation. The molecular weights provided for PAM (Kemira

Co.) and XG (PFP Technology) by the vendors are (6–

8) 9 106 kg mol-1 and (4–5) 9 106 kg mol-1, respec-

tively. The accurate values for molar mass were measured

using light scattering (for HPAM) and viscometry (for XG)

methods. In the light scattering experiments, all solvents

were filtered through 0.02 lm cellulose acetate Millipore

filters. The HPAM solutions were prepared by dissolution

of a known amount of polymer in the 0.5 mol L-1 NaCl

solvent. The solutions were filtered through a 0.45 lm cellulose acetate Millipore filters. A concentration range of

the polymer solutions (0.2–2.0 g L-1) were analyzed using

the batch mode (without size separation) of a multi-angle

light scattering (MALS) detector (DAWN-HELEOS II,

Wyatt Technology) with a laser wavelength of 658 nm.

The specific refractive index increments (dn/dc) value of

the HPAM in 0.5 mol L-1 NaCl solution, which was

determined by an OPTILAB T-reX differential refrac-

tometer (Wyatt Technology) at 633 nm and 25 C, was 0.162 mL/g. Viscosity averaged molecular weight of XG

was measured using the method described in the literature

(Sohn et al. 2001). In this method, the intrinsic viscosity [g] was measured with an Ubbelohde capillary viscometer

(diameter capillary 0.46 mm, Schott-Gerate), immersed in

a water bath maintained at 25.0 ± 0.1 C. First, the

specific viscosity gsp was calculated from the relative vis-

cosity, which is the ratio of the viscosity of xanthan gum

solution at a certain concentration to that of the solvent.

Each concentration was measured five times. The plot of

gsp/C versus C (C is the concentration of solutions) gave a

straight line, the intercept of which was [g]. Then, using the Mark–Houwink equation the molar mass was calculated:

g½ ¼ lim c!0

gsp c

1:35 ½mL/g ð1Þ

The measured values for the molecular weights of the

polymers, HPAM and XG, were 7.2 9 106 kg mol-1 and

3.9 9 106 kg mol-1, respectively.

To establish a baseline for further studies, deionized

water was used throughout. Using an analytical balance,

polymer powders were weighed with an accuracy of

±1 mg (Mettler Toledo XS603s). The preparation of the

polymer solutions took place in a separate tank. First, the

polymer powders were gradually sprinkled into the solvent

and slowly agitated at 30 rpm, in order to prevent particles

from clumping on the surface. Then the prepared solutions

were stored overnight for complete hydration. The studied

concentrations of HPAM solutions were 100, 150, 200,

500, and 1000 wppm. In order to investigate the effect of

XG, mixed polymer solutions of 100 wppm

HPAM ? 100 wppm XG (total C = 200 wppm), 150

wppm HPAM ? 100 wppm XG (total C = 250 wppm),

and for comparison, 600 wppm XG solutions were

prepared.

A closed-loop flow system was used for drag reduction and

turbulent flow measurements (Fig. 1). The system is

comprised of a 60-L supply tank connected to a progressive

cavity pump (SEEPEX BN 10-12) with a pumping capacity

of 30 GPM (113.56 L/min), and a seamless stainless steel

horizontal pipe test section of L = 8 ft. (2.44 m) and inner

diameter of 1 in. (2.54 cm). The flow rate of the system

was measured using a mass flow meter (OPTIMASS 1000,

KROHNE) with an accuracy of ±0.15% and a repeatability

of ±0.05% as stated by the manufacturer. The pressure

drop data along the measuring length of the pipe were

gathered using a membrane differential pressure transducer

(PX409, OMEGA). At each flow rate, the Fanning friction

factor is calculated by:

ð2Þ

Here, f is the Fanning friction factor, q is the fluid density,

U is the average velocity, DP is pressure drop in the

measurement length of L, and D is the internal diameter of

the pipe.

the polymer solutions was defined as:

DR ¼ fw fs

where subscripts ‘‘w’’ and ‘‘s’’ stand for water and polymer

solution, respectively, and ‘‘Re = const.’’ signifies the fact

that the comparison between the flows is made at the same

Reynolds numbers. Here Re = qUD/ga, and ga is fluid

viscosity. In drag reduction experiments, the flow rate was

increased stepwise (and kept constant for 1 min at each

flow rate), and then, the polymer solutions were sheared in

the flow loop at maximum flow of 30 GPM for 2 h and

sampling was performed eight times at shearing periods of

t = 0, 15, 30, 45, 60, 80, 100, and 120 min. After the

shearing process, the flow rate was decreased stepwise in

the same manner as it was increased.

Viscosity measurements were carried out in a DHR

controlled stress rheometer. The instrument is equipped

with a Peltier system to control sample temperature. In our

experiments, sample temperature was maintained at

25 ± 0.01 C. The geometry used in the apparent viscosity

414 Pet. Sci. (2017) 14:412–423

123

angle were 60 mm and 2, respectively. Approximately,

2 mL of the solution was placed between the cone (rotating

plate) and the fixed plate and the instrument was set to the

strain control mode. In this mode, shear rate ( _c) was log-

arithmically increased from 0.01 to 1000 s-1 and shear

stress was measured simultaneously, and then, apparent

viscosity was calculated using ga ¼ r= _c correlation, where r and ga are shear stress and apparent viscosity, respec-

tively. The power-law and Carreau–Yasuda viscosity

models were used for fitting the viscosity data.

In the power-law model, n (behavior index) is a measure

of deviation from Newtonian behavior and K (consistency

index) is a measure of average viscosity. K and n known as

power-law parameters were used in friction factor

calculations.

ga ¼ Kð _cÞn1 ð4Þ g g1 g0 g1

¼ 1þ ðk _cÞa½ n1 a ð5Þ

In the Carreau–Yasuda equation, g is the shear viscosity, and g0 and g? are viscosities at zero-shear and infinite-

shear plateaus, while k, n, and a represent the inverse shear

rate at the onset of shear thinning, power-law index, and

transition index, respectively.

3.1 Polyacrylamide solutions

In order to assess the degree of drag reduction and polymer

degradation, several samples were taken at specified

intervals over the shearing process. Shear stress and

apparent viscosity of the samples were measured in the

rheometer, and the power-law and Carreau–Yasuda

parameters were calculated. For Newtonian fluids, the

value of n is 1 and for shear-thinning fluids, such as

polymer solutions, n is\1. As the value of n deviates from

1, the degree of non-Newtonian behavior increased. The

Carreau–Yasuda and power-law parameters calculated for

different concentrations of the anionic polyacrylamide are

shown in Table 1 and Fig. 2a, b, respectively. Comparison

of power-law parameters of fresh (zero shearing time)

HPAM solutions showed that by increasing concentration,

values of K increased and n values decreased, indicating

increased non-Newtonian behavior. It can also be found

that, as the shearing time increased, the values of power-

law parameters changed for all the polymer solutions.

Figure 2a shows that, over the shearing time, K values of

HPAM solutions decreased and n values increased and get

close to one (Newtonian behavior). The difference in the

n values of the solutions before and after the shearing was

P

Data acquisition and control

Fig. 1 Schematic illustration of the flow loop; instrumentation consists of a digital flow meter (F), differential pressure transducer (P), valves

(V), and temperature sensors (T)

Pet. Sci. (2017) 14:412–423 415

123

overall change in n values (after the shearing period) was

35% for a 100 wppm solution, and by increasing concen-

tration, the maximum change in n values (152%) appeared

at 200 wppm. As the concentration increased above

200 wppm, n droped to 69% for the 1000 wppm solution.

As a result of shear degradation and consequently viscosity

reduction, K values declined. By increasing concentration

from 100 wppm to 1000 wppm, K values reached a max-

imum decline of 64% at 200 wppm, but with further con-

centration increase a 33% decline in K value was found for

1000 wppm HPAM solution.

Fig. 3, where the apparent viscosity of the 200 wppm

HPAM solution, at shear rates under 10 s-1, undergoes

drastic reduction as the circulation time increases. The

reason that we only saw changes at lower shear rates might

be related to the scission of the molecules that belong to the

high tale of the molecular weight distribution of the

polymer (Liberatore et al. 2004). Those molecules con-

tributed to the formation of the zero-shear viscosity

plateau.

Prandtl–Karman coordinates are a semilog graph of f -

versus Re.f, where f and Re are Fanning friction factor and

Reynolds number, respectively. Using Prandtl–Karman

Table 1 Parameters of

Carreau–Yasuda model for

HPAM, XG, and HPAM/XG

solutions

Concentration of solution g0, Pa s g?, Pa s k, s a n

100 wppm HPAM 0.0835 0.0035 4.96 1.37 0.37

150 wppm HPAM 0.2668 0.0041 5.46 3.15 0.26

200 wppm HPAM 0.3717 0.0042 5.80 3.14 0.27

500 wppm HPAM 1.2105 0.0052 8.70 3.74 0.26

1000 wppm HPAM 3.5071 0.0067 10.1 3.52 0.21

600 wppm XG 0.2689 0.0040 5.34 1.92 0.43

100 wppm HPAM ? 100 wppm XG 0.1331 0.0039 4.18 2.51 0.36

150 wppm HPAM ? 100 wppm XG 0.2873 0.0038 7.2 2.28 0.33

0

0.1

0.2

0.3

0.4

0.5

0.6

0.7

0.8

0.9

P ow

er -la

w in

de x

100 wppm

150 wppm

200 wppm

500 wppm

1000 wppm

Time, min

K , P

a· sn

Time, min

Fig. 2 Power-law model parameters variation over shearing time for HPAM solutions

1

10

100

1000

0.01 0.1 1 10 100 1000

Sample 1 Sample 2 Sample 3 Sample 4 Sample 5 Sample 6 Sample 7 Sample 8

η a , m

Fig. 3 Apparent viscosity of 200 wppm sheared HPAM samples

(samples 1–8: fresh, 15, 30, 45, 60, 80, 100, and 120 min shearing

time)

123

coordinates, the degree of DR of polymer solutions can be

compared with respect to the boundaries of drag reduction;

the onset of drag reduction as the point of departure from

Prandtl–Karman law and maximum drag reduction (MDR)

or Virk’s asymptote (White and Mungal 2008; Virk 1975).

Prandtl–Karman plot for different concentrations of HPAM

is shown in Fig. 4. Three flow regimes can be detected:

(a) Re ffiffiffi f

obey Poiseuille’s law.

p \350; laminar to turbulent transition.

(c) Re ffiffiffi f

p [ 350; turbulent flow.

It is observed that except for the laminar to turbulent

transition region, the turbulent friction factor data for the

solutions are bounded in the area between the two universal

asymptotes and the data points are linear for all

concentrations.

Results of linear fitting of the data points in the turbulent

region (Table 2) revealed that by increasing the concen-

tration of polymer, the slope of the lines tended to increase.

According to the literature, the slope increment with

respect to the Prandtl–Karman law (d) is proportional to the

square root of polymer concentration (d / ffiffiffiffi C

p ) with a

values are reported in Table 2. The proportionality constant

for the HPAM used in this work is calculated to be

0.27 ± 0.05. Figure 4 shows that by increasing HPAM

concentration, the extent of DR increases and the data

points approach Virk’s asymptote. Among different con-

centrations, the extent of DR and slope of data points for

100 wppm HPAM solution were closest to the Prandtl–

Karman line (the onset of DR). On the other hand, the

greatest DR belongs to the 1000 wppm solution. For

solutions with polymer content greater than 200 wppm, in

200\Re ffiffiffi f

p \500 range, the data points were nearly tan-

gential to the MDR line, but by increasing the flow rates

(Reynolds number), the data points tended to deviate from

MDR. Results indicated that further increase in concen-

tration did not have a large effect on the degree of DR in

the experimental conditions of this work.

The effect of polymer concentration and mechanical

degradation on the Fanning friction factor of HPAM

solutions is shown in Fig. 5a, b, respectively. It can be seen

that even at low concentrations of polymer (100 wppm),

Fanning friction factor values were much lower than those

of water. Increasing polymer concentration resulted in

further reduction in friction factors (data points get close to

the maximum drag reduction asymptote), and conse-

quently, drag reduction efficiency increased. The smallest

values of friction factors at different Reynolds numbers

belong to 1000 wppm solution. It was also observed that

the difference between turbulent friction factors of 200,

500, and 1000 wppm solutions was very small, which is in

agreement with the results shown in Prandtl–Karman

coordinates, indicating that at the studied range of Rey-

nolds numbers, DR efficiency was close to its maximum

value (MDR); further increase in concentration did not

change friction factors. We can also observe that as the

Reynolds numbers increased, the data points tended to

deviate from MDR.

Shearing had a large impact on reducing the DR ability

of polyacrylamide solutions. Comparing the friction factors

of 200 wppm HPAM solution at different Reynolds num-

bers (Fig. 5b) showed a 30%–50% decline after 2 h of

shearing. It can be observed that as a result of shearing,

friction factor values moved away from MDR line and

shifted toward water friction factors at different Reynolds

numbers. Although flow rate was constant for all the

experiments, a shift in the data points of the sheared

samples toward lower Reynolds numbers was observed.

0

5

10

15

20

25

100 wppm-Fresh 150 wppm-Fresh 200 wppm-Fresh 500 wppm-Fresh 1000 wppm-Fresh

Poiseuille’s law

Fig. 4 Prandtl–Karman coordinates for HPAM solutions

Table 2 Linear fit results of

turbulent regime Concentration, wppm Linear fit equation R2 Slope increment (d)

100 1= ffiffiffi f

p ¼ 6:0 logRe

123

The shift was an indication of alteration in the flow regime,

which occurred due to the change in the rheological

properties of the solutions as a result of shear degradation.

Figure 6 shows the changes in the DR% over shearing time

for different concentrations of HPAM at constant flow rate.

It was observed that, for fresh samples (t = 0), the extent

of DR increased from 30% to 67% by increasing polymer

concentration from 100 to 1000 wppm. Results also indi-

cated that solutions above 200 wppm produced nearly

identical DR at the early stages of shearing (t\ 20 min),

which corresponds to the results shown in Prandtl–Karman

coordinates (Fig. 4). But beyond 20 min, the DR curves

tended to diverge, indicating that the degree of shear

degradation was different for each polymer concentration.

Ptasinski et al. (2003) reported that in flexible polymers

such as HPAM, as shear force reached a certain level, the

molecules stretch and consequently effective viscosity

increased, the turbulent buffer layer thickened, and due to

dissipation of the energy from turbulent fluctuations drag

was reduced. It is also known that drag is reduced when

turbulent flow interacts with polymer networks. When

polymer concentration is high enough (above critical

overlap concentration, C*), polymer chains are packed

closer and begin to interact with each other and form

entangled networks (Skelland and Meng 1996).

The decline in the degree of DR was observed at all the

concentrations of HPAM solution. Resistance to mechani-

cal degradation over the shearing period is shown in Fig. 7.

Results showed that, as the concentration increased, the

resistance to mechanical degradation also increased. This

made the 100 wppm solution the least resistant and

1000 wppm solution the most resistant to mechanical

degradation. These results agreed with those reported by as

Soares et al. (2015), indicating that increasing polymer

concentration (PAM or PEO) in the solution could increase

the resistance to mechanical degradation. It was also

observed that the shear stabilities of 100, 150, 200 wppm

solutions were very close and followed the same trends. In

other words, 200 ppm solution was only slightly more

resistant to degradation (DRt=120/DRmax = 0.5) than

Fr ic

tio n

fa ct

0.1(a) (b)

Fig. 5 Friction factor versus Re: a effect of HPAM concentration and b effect of shearing on 200 wppm HPAM

0

10

20

30

40

50

60

70

80

% D

100 wppm 150 wppm 200 wppm 500 wppm 1000 wppm

MDR

Fig. 6 %Drag reduction for different concentrations of HPAM at

30 GPM (113.56 L/min)

123

100 wppm solution (DRt=120/DRmax = 0.39). But, above

200 wppm a sudden rise in the shear resistance of the

solutions was observed. Both 500 and 1000 wppm solu-

tions showed superior shear stability compared to other

solutions. We found that although 200 wppm HPAM

solution had similar initial DR% to 500 and 1000 wppm

solutions (Fig. 6), it had a larger decline in DR (Fig. 7).

The values of DRt=120/DRmax for 500 and 1000 wppm

solutions were 0.62 and 0.72 at the end of 2-h shearing

period, respectively. It is also interesting to note that the

DR/DRmax declined at a slower rate after t = 60 min. For

example, the reduction in DR/DRmax value for 1000 wppm

solution from t = 60 min to t = 120 min was only 0.06.

From viscosity measurements, the critical overlap con-

centration (the concentration that marks the beginning of

polymer–polymer interaction) of the HPAM solution was

determined to be 200 wppm. At C\ 200 wppm, there was

no polymer network, so there was no decline due to

polymer network breakup, but at C[ 200 wppm, the net-

works were more entangled and upon deformation can

recover quickly. Also, it seems that at higher concentra-

tions (C[ 200 wppm), the extensional force from the

turbulent flow was distributed among a larger number of

molecules, which resulted in a lower number of chain

scissions and higher DR stability. But at C\ 200 wppm

polymer networks just began to form and were weak.

Therefore, at the beginning of the shearing process DR

efficiency increased, but gradually as shear forces acted,

unstable polymer networks, as well as individual polymer

molecules broke up, which resulted in a large decline in the

DR efficiency of C\ 200 wppm HPAM solutions com-

pared to higher concentrations.

Another result was that the rate of DR decline was fast

in the first 60–80 min of the shearing process. This is

probably due to the presence of longer chains of polymer in

the fresh solutions, which are more susceptible to chain

scissions (require less energy to break). After 60 min, the

gap between DR lines (Fig. 6) remained nearly constant,

which indicated that polymer chains were broken up at a

similar rate at all the concentrations.

Several models for correlating the DR behavior of

polymer solutions can be found in the literature. Two of the

most common models are the exponential decay model

(Bello et al. 1996) and Brostow’s model (Brostow 1983).

Based on the exponential decay model proposed by Bello

et al. (1996), DR follows an exponential decline with time

for polyacrylamide and polysaccharide solutions:

DR% tð Þ=DR% 0ð Þ ¼ e t=kð Þ ð6Þ

where DR% (t) and DR% (0) (or DRmax) are percent drag

reduction at times t and t = 0, respectively, and k is an

adjustable parameter. Brostow’s equation is a more general

model, which has been applied to various shear degradation

applications (Lim et al. 2003) and has been developed to

quantitatively describe DR and its changes with time:

DR% tð Þ=DR% 0ð Þ ¼ ½1þWð1 e htð ÞÞ1 ð7Þ

Here W is the average number of vulnerability points per

chain and h is called rate constant.

The two models were used in this work to correlate the

DR data of HPAM and HPAM/XG solutions. Calculated

model parameters and goodness of fit (R2) for both models

are reported in Table 3. The solid lines in Fig. 6 represent

the fitting results. It can be found that for the studied

concentrations of HPAM solution, both models describe

the degradation behavior well, though Brostow’s model

gives better fits and its predicted values are more accurate.

0

0.1

0.2

0.3

0.4

0.5

0.6

0.7

0.8

0.9

1.0

100 wppm 150 wppm 200 wppm 500 wppm 1000 wppm

Time, min

D R

/D R

m ax

solutions at 30 GPM (113.56 L/min)

Table 3 Parameters of Brostow

and exponential decay models

k, min R2 W h, min-1 R2

100 87.32 0.96 374.2 32.7e-5 0.94

150 146.7 0.97 43.43 2.3e-4 0.98

200 162.3 0.95 2.723 3.9e-3 0.99

500 245.0 0.90 0.8628 9.6e-3 0.98

1000 312.1 0.88 0.6351 8.1e-3 0.96

Pet. Sci. (2017) 14:412–423 419

123

In order to verify the possibility of stabilizing HPAM with

XG, mixed solutions were prepared and sheared in the

same manner as the HPAM solutions. Based on the results

obtained from the previous section, the DR behavior of

binary polymer solutions was compared to that of

200 wppm HPAM solution. Several authors have men-

tioned that the degree of DR in XG solutions depends on

the concentration and molar mass of XG (Soares et al.

2015; Pereira et al. 2013). So higher concentrations of XG

are required to reach the same level of DR as HPAM. Our

preliminary experiments showed that the DR efficiency of

600 wppm XG was close to the DR values of 200 wppm

HPAM.

solutions and solutions of 600 wppm XG and 200 wppm

HPAM are shown in Fig. 8a. It was found that, although

polymer concentration in the 600 wppm XG solution was

greater than that of 200 wppm HPAM solution, the

600 wppm XG solution possessed greater friction factors.

Higher flexibility of HPAM polymer chains with respect to

semirigid XG chains resulted in higher energy adsorption

(stretching) due to interaction with dynamic turbulent flow

and subsequently, superior drag reduction capability of

flexible polymers. Also, it was found that in the fresh

binary solutions, there is no outstanding synergetic effect

between HPAM and XG molecules. Even the 150 wppm

HPAM ? 100 wppm XG solution, which has a higher total

polymer concentration, showed larger friction factors than

200 wppm HPAM.

after 120 min of shearing. Because of high shear stability,

XG solution maintained its initial friction reduction

0.001

0.01

0.1

0.003

0.03

(a)

(b)

Fig. 8 Fanning friction factor of mixed solutions in a fresh form and b after shearing for 120 min

420 Pet. Sci. (2017) 14:412–423

123

efficiency, with a relatively small change in friction factor

values. But for the mixed HPAM/XG solutions, the friction

factor values largely increased as a result of shearing. It is

interesting to note that 200 wppm HPAM solution had a

larger increase in its friction factors than mixed solutions

(Fig. 8b). This suggested that addition of XG was benefi-

cial in controlling the shear degradation of HPAM. The

decline in the DR efficiency and shear resistance of the

samples over shearing time is shown in Figs. 9 and 10.

Also, as mentioned above, Brostow’s and exponential

decay models were used to correlate DR with time (solid

lines in Fig. 9; Table 4).

The results indicated that the DR efficiencies of both

HPAM and XG binary solutions were smaller than that of

200 wppm HPAM solution, indicating that partially

replacing HPAM with XG in the binary solutions had

reduced the DR efficiency of the single HPAM solution.

Regarding the DR behavior of HPAM/XG binary mixtures,

different views can be found in the literature. Sandoval and

Soares (2016) recently reported that the DR efficiency of

HPAM/XG mixture is close to the DR values of the single

HPAM solution at the same total concentration. However,

they confirmed that the synergetic effect in PAM/XG

mixture is not as notable as PEO/XG. Reddy and Singh

(1985) also studied PAM/XG mixtures and reported that

the single PAM solution has a higher DR efficiency than a

binary mixture. Their data were limited to fresh solutions.

We believe that the differences in the reported data might

be attributed to the differences in the experimental condi-

tions. In our work, since we were dealing with two nega-

tively charged polymers in the solution, we would expect

to obtain different results. We also believed that due to the

higher flexibility (higher molecular weight) of the anionic

HPAM used in our experiments, HPAM molecules were

more susceptible to scission and the interaction between

HPAM and XG was reduced. Compared to 600 wppm XG

solution, the DR% of 100 wppm HPAM/150 wppm XG

solution was high only in the first 60 min of the shearing

process and after that, as a result of mechanical degradation

the DR values declined. Also, it was found that the

100 wppm HPAM/100 wppm XG solution was less effi-

cient in DR than the 600 wppm XG solution from the

beginning till end of the shearing period. Comparison of

the shear resistance (DR/DRmax) of the solutions revealed

that, as expected, 600 wppm XG solution had the best

shear stability among all the solutions and the least decline

in DR over the shearing period (0.15 decline in DR/DRmax

value). Contrary to XG, 200 wppm HPAM and the binary

HPAM/XG solutions suffered from poor shear resistance

and a large decline in their DR efficiencies. These results

are in agreement with the results reported by Sandoval and

Soares (2016). It is interesting to note that the shear

resistance of both binary solutions and 200 wppm HPAM

solution was nearly identical.

% D

n

Time, min 200 wppm HPAM 600 wppm XG 100 wppm HPAM + 100 wppm XG 150 wppm HPAM+100 wppm XG

MDR

Fig. 9 %Drag reduction for mixed HPAM/XG solutions at 30 GPM

(113.56 L/min)

% D

n

Time, min 200 wppm HPAM 600 wppm XG 100 wppm HPAM + 100 wppm XG 150 wppm HPAM+100 wppm XG

Fig. 10 Effect of shearing on DR decline for mixed HPAM/XG

solutions

and exponential decay models

for mixed HPAM/XG solutions

k, min R2 W h, min-1 R2

200 (HPAM) 145 0.92 1.792 6.8e-3 0.99

600 (XG) 571 0.94 0.3853 8.8e-3 0.96

100 (HPAM) ? 100 (XG) 137 0.92 44.49 2.2e-4 0.96

150 (HPAM) ? 100 (XG) 127 0.89 1.768 8.4e-3 0.99

Pet. Sci. (2017) 14:412–423 421

123

inferred that addition of XG reduced the DR capability of

mixed solutions (DR% = 40% and 55%) with respect to

200 wppm HPAM solution. Also results suggested that

increasing HPAM concentration in the mixed solutions

does not change the DR efficiency decline significantly.

Since there was only a small amount of chain degradation

in semirigid polymers, the extent of DR depended only on

the interaction between polymer chains and entanglements,

which is directly related to polymer concentration. It

should be considered that the concentration of XG was

100 wppm for mixed solutions, which is below the critical

concentration of XG (C* & 300 ppm). Hence, as sug-

gested by other authors (Wyatt et al. 2011; Berman 1978),

mixing HPAM with higher concentrations of XG would be

more beneficial in maintaining high DR efficiency and

even better control of shear degradation of polyacrylamide

solutions, which is the subject of our future work. Same as

for the HPAM solutions, Brostow and exponential decay

models were used to correlate the drag reduction behavior

over time for the HPAM/XG mixed solutions. The result is

shown in Fig. 9 and Table 4. It can be found that both

models give good fitting, but similar to HPAM solutions,

the Brostow’s model correlated the DR reduction data

better.

concentrations of HPAM, 1000 wppm solution has the

highest drag reduction efficiency and the lowest decline in

DR%. Increasing the concentration above 200 wppm does

not change the DR% of the fresh samples significantly,

though increasing concentration increases resistance to

mechanical degradation. Results also indicate that mixing

flexible HPAM with XG did not improve the degree of DR

significantly, but slightly improved the DR stability of

HPAM solutions. Since the drag reduction of rigid poly-

mers depends only on concentration, mixing HPAM with

higher concentrations of XG might be beneficial in main-

taining the DR efficiency of HPAM as well as improving

its shear stability. Brostow and exponential decay models

were used to correlate the drag reduction decline data.

Results indicate that both models can correlate the DR

behavior of HPAM, as well as mixed HPAM/XG solutions.

Brostow’s model gave slightly better fits.

Acknowledgements The authors would like to thank the Research

Partnership to Secure Energy for America (RPSEA) and Oklahoma

State University Chemical Engineering Department for partial support

of this project.

Open Access This article is distributed under the terms of the

Creative Commons Attribution 4.0 International License (http://crea

tivecommons.org/licenses/by/4.0/), which permits unrestricted use,

distribution, and reproduction in any medium, provided you give

appropriate credit to the original author(s) and the source, provide a

link to the Creative Commons license, and indicate if changes were

made.

References

Barati R, Liang J-T. A review of fracturing fluid systems used for

hydraulic fracturing of oil and gas wells. J Appl Polym Sci.

2014;131(16). doi:10.1002/app.40735.

Bello JB, Muller AJ, Saez AE. Effect of intermolecular cross links on

drag reduction by polymer solutions. Polym Bull.

1996;36(1):111–8. doi:10.1007/BF00296015.

Berman NS. Drag reduction by polymers. Annu Rev Fluid Mech.

1978;10(1):47–64.

solutions in flow. Polymer. 1983;24(5):631–8.

Bunger AP, McLennan J, Jeffrey R. Effective and sustainable

hydraulic fracturing. InTech, Janeza Trdine. 2013;9:51000.

Campolo M, Simeoni M, Lapasin R, Soldati A. Turbulent drag

reduction by biopolymers in large scale pipes. J Fluids Eng.

2015;137(4):041102.

AIChE J. 1974;20(6):1222–4.

Rheol Acta. 1978;17(4):426–32.

crosslinked fracturing fluids. 1 January 2012. SPE: Society of

Petroleum Engineers; 2012.

Kaufman PB, Penny GS, Paktinat J. Critical evaluation of additives

used in shale slickwater fracs. 1 January 2008. SPE: Society of

Petroleum Engineers; 2008.

hydrodynamic degradation of polysaccharides and synthetic

polymers. J Appl Polym Sci. 1971;15(3):607–18.

Kim CA, Choi HJ, Kim CB, Jhon MS. Drag reduction characteristics

of polysaccharide xanthan gum. Macromol Rapid Commun.

1998;19(8):419–22. doi:10.1002/(SICI)1521-

3927(19980801)19:8\419:AID-MARC419[3.0.CO;2-0.

Kulmatova D. Turbulent drag reduction by additives. Phys Rev Lett.

2013;84:4765–8.

Larch KL, Aminian K, Ameri S. The impact of multistage fracturing

on the production performance of the horizontal wells in shale

formations. 1 January 2012. SPE: Society of Petroleum Engi-

neers; 2012.

Liberatore MW, Baik S, McHugh AJ, Hanratty TJ. Turbulent drag

reduction of polyacrylamide solutions: effect of degradation on

molecular weight distribution. J Nonnewton Fluid Mech.

2004;123(2):175–83.

Lim S, Choi H, Lee S, So J, Chan C. k-DNA induced turbulent drag

reduction and its characteristics. Macromolecules.

2003;36(14):5348–54.

Loveless D, Holtsclaw J, Weaver JD, Ogle JW, Saini RK.

Multifunctional boronic acid crosslinker for fracturing fluids.

19 January 2014. IPTC: International Petroleum Technology

Conference; 2014.

Malhotra J, Chaturvedi P, Singh R. Drag reduction by polymer–

polymer mixtures. J Appl Polym Sci. 1988;36(4):837–58.

422 Pet. Sci. (2017) 14:412–423

extensional and turbulent flows. Polym Commun. 1984;25(5):

144–6.

Moussa T, Tiu C. Factors affecting polymer degradation in turbulent

pipe flow. Chem Eng Sci. 1994;49(10):1681–92.

Palisch TT, Vincent M, Handren PJ. Slickwater fracturing: food for

thought. SPE Prod Oper. 2010;. doi:10.2118/115766-PA.

Pereira AS, Andrade RM, Soares EJ. Drag reduction induced by

flexible and rigid molecules in a turbulent flow into a rotating

cylindrical double gap device: comparison between Poly

(ethylene oxide), Polyacrylamide, and Xanthan Gum. J Nonnew-

ton Fluid Mech. 2013;202:72–87. doi:10.1016/j.jnnfm.2013.09.

008.

Ptasinski P, Boersma B, Nieuwstadt F, Hulsen M, Van den Brule B,

Hunt J. Turbulent channel flow near maximum drag reduction:

simulations, experiments and mechanisms. J Fluid Mech.

2003;490:251–91.

Reddy G, Singh R. Drag reduction effectiveness and shear stability of

polymer–polymer and polymer–fibre mixtures in recirculatory

turbulent flow of water. Rheol Acta. 1985;24(3):296–311.

Rodriguez F, Winding C. Mechanical degradation of dilute poly-

isobutylene solutions. Ind Eng Chem. 1959;51(10):1281–4.

doi:10.1021/ie50598a034.

Sandoval GA, Soares EJ. Effect of combined polymers on the loss of

efficiency caused by mechanical degradation in drag reducing

flows through straight tubes. Rheol Acta. 2016;55(7):559–569.

Skelland A, Meng X. The critical concentration at which interaction

between polymer molecules begins in dilute solutions. Polym

Plast Technol Eng. 1996;35(6):935–45.

Soares EJ, Sandoval GA, Silveira L, Pereira AS, Trevelin R, Thomaz

F. Loss of efficiency of polymeric drag reducers induced by high

Reynolds number flows in tubes with imposed pressure. Phys

Fluids (1994–present). 2015;27(12):125105.

Sohn J-I, Kim C, Choi H, Jhon M. Drag-reduction effectiveness of

xanthan gum in a rotating disk apparatus. Carbohydr Polym.

2001;45(1):61–8.

Virk P, Baher H. The effect of polymer concentration on drag

reduction. Chem Eng Sci. 1970;25(7):1183–9.

Virk PS. Drag reduction fundamentals. AIChE J. 1975;21(4):625–56.

doi:10.1002/aic.690210402.

White CM, Mungal MG. Mechanics and prediction of turbulent drag

reduction with polymer additives. Annu Rev Fluid Mech.

2008;40:235–56.

Wu Q, Sun Y, Zhang H, Ma Y, Bai B, Wei M. Experimental study of

friction reducer flows in microfracture during slickwater frac-

turing. 8 April 2013. SPE: Society of Petroleum Engineers;

2013.

ness of dilute and entangled xanthan in turbulent pipe flow.

J Nonnewton Fluid Mech. 2011;166(1–2):25–31. doi:10.1016/j.

jnnfm.2010.10.002.

Abstract

Introduction

Results and discussion